Laboratory for Advanced Electron and Light Optical MethodsCollege of Veterinary Medicine4700 Hillsborough StreetNorth Carolina State UniversityRaleigh, NC 27606Tel: 919-513-6202Fax: 919-513-6464Email: Michael_Dykstra@ncsu.eduwww.cvm.ncsu.edu/research/laelomResin Formulation(For further information, see Dykstra, M.J. and L.E. Reuss. 2003. Biological Electron Microscopy. Theory,Techniques and Troubleshooting, 2 nd Edition. Kluwer Academic/Plenum Publishers, New York)General Cautionary Notes For Resin Formulation:Caution: The chemicals to be mixed can cause contact dermatitis. People with allergies should exerciseparticular caution. Wear neoprene or latex gloves when working with these components, but recognizegloves do not confer complete protection from these chemicals. Work under a fume hood as much aspossible. Vinyl cyclohexene dioxide (a component of Spurr resin) is a known carcinogen. Do NotInhale resin vapors or allow skin contact.Dispose of resins in waste resin jar jar in the fume hoodhood or polymerize the resin to a solidstate before disposal. Never pour resins down the drain. Always wipe lip and cap of bottle beforereclosing it.It is far more accurate to measure by weight than by volume. Take a predried 100 ml Nalgenebottle and add the components carefully, in the order given. After all ingredients have been added, capthe bottle. Mix by inversion for a few minutes.I. Spurr’s Low-Viscosity Embedding Medium (Spurr, A.R. 1969. A low-viscosity epoxy resinembedding medium for electron microscopy. J. Ultrastruct. Res. 26: 31.A. Purpose: This resin formulation, with a viscosity of 60 cp, was developed for infiltration ofplant cells, which are typically harder to penetrate than mammalian cells due to their cellwalls. Because of its low viscosity, infiltration times are relatively short, no specimenrotation is necessary, and almost all samples are well-penetrated with our protocols. Theresin is completely miscible with ethanol, and acetone, though blocks polymerized followingan ethanol-only dehydration series often have a slightly tacky surface, unlike those that havebeen passed through acetone as a transitional solvent. The ethanol-only blocks may also beslightly more brittle during trimming and sectioning. Spurr resin is chemically reactive withsilicone flat-embedding molds and eventually ruins them, unlike other epoxide resins.B. Procedure: Our recipe is modified from those provided by most vendors supplying the resincomponents. We have selected the 6.3 g DER recipe as a compromise allowing thepolymerized blocks to be equally well-sectioned with glass or diamond knives. If only usingglass knives, 6.4 g of DER is the better choice, and if only diamond knives are used, theharder 6.2 g DER recipe is recommended.
1. Add the following components, in the order listed, to a 100 ml Nalgene bottle:ERL 4221*10.0 gD.E.R. 736 6.3 gNSA26.0 gDMAE 0.4 g*ERL 4221 has replaced the carcinogenic component, vinylcyclohexene dioxide,used prior to the year 2005Polymerize samples after infiltration at approximately 70°C for 8 hours to 3 days.Note: Excess resin can be stored by wrapping the Nalgene bottle cap with parafilm andputting in the freezer. It will keep several months. Always bring to room temperaturebefore opening to prevent condensation of water on the resin, as it will prevent properpolymerization.II.SPI-PON 812, a Substitute for EPON 812, which was discontinued by SHELL Oil Co. in1978Purpose: This resin mixture is supposed to be a substitute for EPON 812. This resin has ahigher viscositiy than Spurr resin, so it needs a longer infiltration schedule than Spurr resin. Inaddition, it polymerizes at a lower temperature than Spurr resin and is not reactive with siliconemolds, unlike Spurr resin, which is reactive. The plastic trims and sections easily. SPI-PONstains more readily than Spurr and has a slightly grainy appearance. SPI-PON can be stainedwith 2% aqueous UrAc for about 5 min and for about 8 min in Reynolds’ lead citrate to achievewrinkle-free sections that are a little sharper than Spurr sections stained with methanolic UrAcand lead citrate.A. Procedure:1. Resin Formulation: Add the components in the order listed, with mixing.By WeightBy Volume18.5 g SPI-PON 812 16.2 ml9.3 g DDSA 10 ml10.0 g NMA 8.9 ml0.6 g DMP-30 0.6 mlThe mixture stays usable for about 1 day at room temperature and will remain usableif frozen for up to 6 months. Be sure to cap the storage container tightly and to sealcontainer with Parafilm. After freezing be sure to bring to room temperature beforeopening container. Water will ruin the resin.2. Sample Processing: Everything in the embedding and fixation procedure is the same aswith Spurr resin procedures except for the embedding procedure outlined below:
a. After fixation and dehydration to 100% acetone as described in SOP 6.0.1, placethe samples in in a 1:1 mixture of SPI-PON 812/Acetone at room temperatureforabout 1 hr with gentle stirring.b. Put in 100% SPI-PON 812 for about 1 hr with stirring.c. Put in new 100% SPI-PON 812 for about 1 hr with stirring.d. Put in 100% SPI-PON 812 in molds and cure at approximately 60° C for about24 hrs.e. Cool to room temperature and section.